Disorder in the composite crystal structure of the manganese `disilicide' MnSi~1.73~ from powder X-ray diffraction data
Akselrud, L.; Cardoso Gil, R.; Wagner-Reetz, M.; Grin, Yu.; Acta Crystallographica Section B 71 (2015) 707–712; doi:10.1107/S2052520615019757

data_2107283
_publ_section_title
;
 Disorder in the composite crystal structure of the manganese `disilicide'
 MnSi~1.73~ from powder X-ray diffraction data
;
_journal_coeditor_code           KC5025
_journal_issue                   6
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              707
_journal_page_last               712
_journal_paper_doi               10.1107/S2052520615019757
_journal_volume                  71
_journal_year                    2015
_chemical_formula_sum            'Mn2 Si3.5'
_space_group_IT_number           141
_space_group_ssg_name            'I 41/a m d(00p)00ss'
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-I 4bd 2'
_symmetry_space_group_name_H-M   'I 41/a m d :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.5235(3)
_cell_length_b                   5.5235(3)
_cell_length_c                   4.3634(3)
_cell_measurement_temperature    295.0
_cell_modulation_dimension       1
_cell_subsystems_number          2
_cell_volume                     133.123(14)
_computing_cell_refinement       WinCSD
_computing_data_reduction        WinCSD
_computing_publication_material  'WinCSD (Akselrud et al, 1993)'
_computing_structure_refinement  WinCSD
_computing_structure_solution    WinCSD
_diffrn_ambient_temperature      295
_diffrn_detector                 'imaging plate'
_diffrn_measurement_device_type  'Huber Guinier G670'
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Cu K\a~1~'
_diffrn_radiation_wavelength     1.54061
_diffrn_reflns_limit_h_max       5
_diffrn_reflns_limit_h_min       0
_diffrn_reflns_limit_k_max       3
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       5
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_theta_max         50.4
_diffrn_source                   'sealed X-ray tube'
_diffrn_source_current           30
_diffrn_source_target            Cu
_diffrn_source_type              'GE ID-3003'
_diffrn_source_voltage           40
_exptl_absorpt_coefficient_mu    89.62
_exptl_crystal_colour            'Grey metallic'
_exptl_crystal_density_diffrn    5.2130
_exptl_crystal_F_000             198.7
_pd_meas_2theta_range_inc        0.005
_pd_meas_2theta_range_max        100.3
_pd_meas_2theta_range_min        15.0
_pd_meas_scan_method             step
_pd_proc_ls_profile_function     pseudo-Voit
_pd_proc_ls_prof_R_factor        0.1123
_pd_proc_ls_prof_wR_factor       0.0870
_pd_spec_mounting                'packed powder pellet'
_pd_spec_size_axial              25
_pd_spec_size_equat              25
_pd_spec_size_thick              1
_refine_ls_goodness_of_fit_all   1.02
_refine_ls_matrix_type           fullcycle
_refine_ls_number_parameters     0
_refine_ls_number_reflns         52
_refine_ls_shift/su_max          0.032
_refine_ls_weighting_details     1/sqrt[Y~i~]
_refine_ls_weighting_scheme      calc
_cod_data_source_file            kc5025sup1.cif
_cod_data_source_block           I
_cod_depositor_comments
;
The following automatic conversions were performed:

'_refine_ls_weighting_scheme' value 'Calc' changed to 'calc'
according to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/IUCr/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 4268 2015-11-12 08:31:59Z antanas 
;
_cod_original_cell_volume        133.13(2)
_cod_database_code               2107283